Microstructures
microstructj.com

Open AccessResearch Article

^{1}

^{2}Faculty of Materials and Manufacturing,

^{3}

Correspondence Address: Prof. Yang Yang, Beijing National Laboratory for Condensed Matter Physics, Institute of Physics, Chinese Academy of Sciences, P. O. Box 603, Beijing 100190, China. E-mail: yang.yang@iphy.ac.cn ; Prof. Lianchun Long, Faculty of Materials and Manufacturing, Beijing University of Technology, No.100, Pingleyuan, Chaoyang District, Beijing 100124, China. E-mail: longlc@bjut.edu.cn

Views:387 | Downloads:72 | Cited:0 | Comments:0 | :0

© The Author(s) 2021. **Open Access** This article is licensed under a Creative Commons Attribution 4.0 International License (https://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, sharing, adaptation, distribution and reproduction in any medium or format, for any purpose, even commercially, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.

The thermal expansion coefficient is an important parameter of monolayer MoS_{2} that affects the performance of its related optoelectronic devices. To obtain the thermal expansion coefficient of monolayer MoS_{2}, suspended and supported MoS_{2} are systematically investigated using micro-Raman spectroscopy in a temperature range of 77-557 K. Obvious differences in the temperature-dependent evolution of the Raman peaks between suspended and supported MoS_{2} are observed, which result from the thermal expansion coefficient mismatch between MoS_{2} and the substrate. With the help of the finite element method, the thermal strain in suspended and supported MoS_{2} is calculated and used to deduce the thermal expansion coefficient mismatch-induced Raman shift. By matching the simulation and experimental results, the thermal expansion coefficient of MoS_{2} is identified through the numerical inversion calculation. Our results demonstrate that the combination of micro-Raman spectroscopy and finite element simulations is highly effective for identifying the intrinsic thermal expansion coefficient of two-dimensional materials.

Monolayer MoS_{2}, thermal expansion coefficient, Raman spectroscopy, finite element method

Transition metal dichlorides (TMDs) are a large class of two-dimensional layered materials with a natural band gap structure and have attracted increasing attention in the past decade^{[1-3]}. Their intralayer atoms are bound by covalent bonds, while their interlayer atoms are coupled by weak van der Waals force. Each layer of a TMD is three atoms thick, with a triangular or hexagonal transition metal atomic plane sandwiched between two triangular layers of dichloride atoms^{[4,5]}. Monolayer TMDs lack the inversion symmetry of the crystal space group and undergo a transition from an indirect to direct band gap^{[6,7]}. MoS_{2} is a typical TMD material with a bulk indirect band gap of 1.29 eV and a direct band gap of 1.9 eV for monolayer MoS_{2}. MoS_{2} has high carrier mobility and optical absorptivity, which give it promising applications in optoelectronic devices.

As a building block of nanodevices, monolayer MoS_{2} is attached to the substrate in practical applications. The differences in the thermal expansion coefficient (TEC) between the MoS_{2} layer and the substrate causes thermal strain inside the MoS_{2} layer. Because the self-heating effect cannot be avoided during the operation of devices, the thermal strain consequently induced by TEC mismatch should be taken into consideration when studying the electronic and transport properties of devices^{[8,9]}. Thermal strain can affect the performance of devices and even results in cracking failure when it exceeds the bearing limit of MoS_{2}^{[10]}. Therefore, determining the TEC of monolayer MoS_{2} is important for its future application in devices.

However, direct measurement of the TEC of monolayer MoS_{2} is still hindered as it is attached to the substrate. Researchers have performed theoretical calculations to obtain the TEC of MoS_{2}^{[11-14]}. The positive linear TEC of two-dimensional (2D) MoS_{2} was estimated using first-principles based on the quasiharmonic approximation^{[11]}. Ding *et al*.^{[12]} used density functional perturbation theory (DFPT) to calculate the phonon spectra of 2H-MoS_{2} structures. Huang *et al*.^{[13]} proposed a negative-positive crossover in the TEC of monolayer MoS_{2} at 20 K, which was attributed to the competition between the modes with negative and positive Grüneisen parameters.

Raman spectroscopy has been demonstrated to be a powerful tool for studying the microstructure and electronic properties of MoS_{2}, including the layer number, stress, doping and so on^{[15-18]}. In recent years, Raman spectroscopy has also been used to study the thermal parameters of MoS_{2}^{[19]}. Zhang *et al*.^{[20]} obtained the TEC of monolayer MoS_{2} using a combination of theoretical and experimental methods and by characterizing the unique temperature dependence of the Raman peaks with three different substrates. Recently, the TEC of few-layer MoS_{2} was investigated by adopting suspended MoS_{2} as a freestanding sample^{[21]}. However, absolute freestanding MoS_{2} cannot be achieved practically. Even when MoS_{2} is suspended on a hole or a groove, it is very difficult to observe the corresponding free expansion.

To our knowledge, previous studies of TEC have depended either on purely theoretical calculations or a combination of experimental characterization with first-principles modeling. In this work, we propose a new method to determine the TEC of MoS_{2} by combining the temperature-dependent Raman spectroscopy with finite element simulations. First, a systematic Raman study is carried out on suspended MoS_{2}, compared with substrate-supported MoS_{2}, in a temperature range from 77 to 557 K. The finite element method is then used to simulate the thermal strain caused by the TEC mismatch between the substrate and MoS_{2}. The corresponding Raman frequency shift obtained by thermal mismatch is also calculated. By ensuring compatibility between the simulation and experimental results, the TEC of monolayer MoS_{2} is finally achieved by employing a numerical inversion method. Our work presents a simple method for assessing the TEC of monolayer MoS_{2}, which can also be widely applied to study the thermophysical properties of many other 2D materials and thin films.

Monolayer MoS_{2} was obtained using a mechanical exfoliation method that has been demonstrated to be a feasible method for producing 2D materials^{[22]}. This was then transferred onto a 300-nm-thick Si substrate that had been previously cleaned by oxygen plasma. Suspended MoS_{2} was achieved by transferring exfoliated MoS_{2} on periodic microhole arrays that was prefabricated on a SiO_{2}/Si substrate by ultraviolet lithography and reactive ion etching technology. The microholes were 5 µm in diameter and 2 µm in depth. Monolayer MoS_{2} was roughly picked out by its color from optical microscopy and further identified using micro-Raman spectroscopy and atomic force microscopy.

Raman spectra were collected using a confocal micro-Raman spectrometer (Horiba HR Evolution). A solid-state laser with a wavelength of 532 nm was used as the excitation source. The laser beam was focused using a 50× long working distance objective with a numerical aperture of 0.5. The spot size was ~1.5 µm. To avoid the heating effect, the laser power was set to less than 1 mW. The sample was placed inside a cryostat cell (Linkam, THMS 600) and the temperature was changed from 77 to 557 K with an interval of 20 K.

According to the experimental environment of the sample in the low-temperature measurements, the mechanical thermal coupling analysis model was established by the finite element method. Two types of simulation models (supported and suspended MoS_{2}) were built accordingly. As shown in Figure 1A, supported MoS_{2} is fully attached to the SiO_{2} substrate (SUP-MoS_{2}). In contrast, suspended MoS_{2} covers the substrate with a microhole (SUS-MoS_{2}), as shown in Figure 1B. The geometries of the models in the simulation were designed to match the real dimensions of the monolayer MoS_{2} and microhole fabricated. The diameter of the microhole was 5 µm and the periodicity was 8 µm. The thickness of monolayer MoS_{2} was set as 0.7 nm according to a previous study^{[23]}. For the simplicity of the simulations, the thickness of the SiO_{2} layer was set as 100 nm, although the SiO_{2} layer in the real sample was 280 nm thick. The physical properties of SiO_{2} employed in the simulations were adopted from the built-in parameters in the software and are listed in Supplementary Table 1.

Figure 1. Schematic illustration of finite element model for (A) supported and (B) suspended MoS_{2}.

In the modeling process, the mesh density was conventional and the maximum and minimum elements were 0.8 and 0.144 µm, respectively. The SiO_{2} base mapping and sweep function were obtained and the monolayer MoS_{2} was then mapped and swept. A layer of hexahedron meshes was obtained. It was assumed that the heating effect from the laser can be ignored. The sample was only subjected to the heat transfer response from the ambient temperature in the cryostat. In the process of the analysis and calculation, the solid mechanics and heat transfer module were coupled and transient analysis was adopted. The heat flux boundary condition was used in the solid heat transfer module. This convection heat flux can be described by the convection heat transfer equation:

where *q*_{0} represents the heat transfer from the environment to the model, *h* is the heat transfer coefficient, *T*_{ext} is the ambient temperature and *T* is the model temperature.

Figure 2A exhibits the optical image of monolayer MoS_{2} transferred on a prepatterned SiO_{2}/Si substrate with microholes. The typical Raman spectra for suspended and supported monolayer MoS_{2} at room temperature (293 K) and 77 K are presented in Figure 2B, in which two Raman modes can be seen clearly. The mode originates from the in-plane vibration of molybdenum and sulfur atoms, while the mode represents the out-of-plane vibration^{[24]}. Regarding the room-temperature spectrum of supported MoS_{2} (SUP-293 K), the mode is located at ~385.5 cm^{-1}, whereas the mode is at ~404.5 cm^{-1}. The frequency difference between the and modes is smaller than 20 cm^{-1}, demonstrating that it is monolayer MoS_{2}^{[25]}. Moreover, the frequency differences between suspended and supported MoS_{2} are also observed in the room-temperature Raman spectra, which could be attributed to the internal strain caused during sample preparation^{[26]}.

Figure 2. (A) Optical microscopy image of monolayer MoS_{2} transferred on a prepatterned SiO_{2}/Si substrate with 5 μm microholes. (B) Raman spectra of MoS_{2} collected at 77 and 293 K. (Solid lines represent SUP-MoS_{2} and the dotted line represents SUS-MoS_{2}).

In addition to the room-temperature spectra, the Raman spectra of SUP-MoS_{2} and SUS-MoS_{2} collected at 77 K also exhibit differences. It is well known that the binding force from the substrate interferes with the deformation of the MoS_{2} film when the temperature changes because of the difference in the TEC of MoS_{2} and the SiO_{2} substrate. Although the experimental conditions are the same, supported and suspended MoS_{2} are subjected to different strain conditions and the deformation in the microstructure of MoS_{2} is different as a result. Consequently, the corresponding atomic lattice vibration is affected by the substrate. Figure 3 presents the Raman spectra of supported and suspended MoS_{2} at selected temperatures. With increasing temperature, an obvious redshift and broadening of the Raman peaks are observed for both suspended and supported MoS_{2}, which can be attributed to the thermal expansion of the crystal lattice of MoS_{2}^{[27,28]}.

For a more detailed analysis of the difference between suspended and supported MoS_{2}, the Raman spectra presented in Figure 3 were deconvoluted using the Lorentz/Gaussian mixed function. The peak positions of the and modes are plotted as a function of temperature in Figure 4 for comparison. The temperature-dependent evolutions of the frequency shifts for supported and suspended MoS_{2} samples are similar and vary approximately linearly with increasing temperature. It is well known that mechanically exfoliated MoS_{2} is transferred and attached on a substrate by weak van der Waals forces. Therefore, the TEC mismatch between MoS_{2} and the substrate induces biaxial stress into MoS_{2} as the temperature changes and becomes a prominent factor that modulates the frequency shift of the Raman peaks. The Raman frequency evolutions of suspended MoS_{2} demonstrate that the substrate effect is exerted on the MoS_{2} layer as a whole, although the suspended zone of MoS_{2} is not directly in contact with the substrate.

Figure 4. Frequency shifts of (A) and (B) modes of suspended and supported MoS_{2} as a function of temperature. The blue and red lines show the fitting results obtained using a linear equation of temperature.

Moreover, as shown in Figure 4, the temperature evolution of the mode is significantly different from that of the mode. For the mode, the temperature-dependent frequency shift for suspended MoS_{2} is much closer to that of supported MoS_{2}. In sharp contrast, the temperature-dependent evolutions of the mode of suspended MoS_{2} are very different from those of supported MoS_{2}. The temperature dependences of the and modes are fitted using the Grüneisen model^{[29,30]}:

where *ω*_{0} is the frequency at 0 K and *χ* is the temperature coefficient. The temperature coefficients of the mode () are -0.0985 and -0.0129 cm^{-1}/K for suspended and supported MoS_{2}, respectively. For the mode, the temperature coefficients () are -0.00952 and -0.00316 cm^{-1}/K for supported and suspended MoS_{2}, respectively. Remarkably, the of suspended MoS_{2} is just 34.1% of that of supported MoS_{2}. This suggests that the mode is more sensitive to the substrate (or dielectric environment). In addition to the TEC mismatch, charge transfer between the TMD film and the substrate or through interfacial states can also influence the temperature evolution of the peak. Su *et al*.^{[31]} observed the accelerated redshift of the mode of MoS_{2} with increasing temperature, which was attributed to the enhanced charge injection from the substrate into the film and the decomposition of adsorbed contaminants. Through the strong electron-phonon interaction, the electron doping effect leads to frequency shifts of the mode^{[32,33]}. In contrast, the electron doping effect can be ignored in the temperature-dependent mode, which could be used to estimate the thermal strain in monolayer MoS_{2}.

According to the literature, the temperature-dependent Raman frequency shift of freestanding MoS_{2} can be commonly attributed to the thermal expansion of the lattice [Δ*ω*^{E}(*T*)] and the anharmonic effect [Δ*ω*^{A}(*T*)], which changes the phonon self-energy^{[34]}. The intrinsic frequency shift of freestanding MoS_{2} [Δ*ω*_{int}(*T*)] can be written as:

For the temperature-induced frequency shifts of supported MoS_{2}, both common thermal effects and TEC mismatch-induced strains must be taken into consideration. As a result, the frequency shifts of supported MoS_{2} can be expressed as^{[21,34]}:

where Δ*ω*(*T*) can be obtained using the frequency position at certain temperature *T* [*ω*(*T*)], shown in Figure 4 subtracted by the peak position at room temperature *T*_{0} = 293 K [*ω*(*T*_{0})].

The term Δ*ω*^{S}(*T*) represents the TEC mismatch-induced frequency shift, which can be expressed as:

where *β* is the biaxial strain coefficient of Raman modes and and are the temperature-dependent TECs of SiO_{2} and MoS_{2}, respectively. The value of *β* can be taken from the literature^{[35]}.

It is known that Δ*ω*^{E}(*T*) and Δ*ω*^{A}(*T*) are the intrinsic frequency shifts of MoS_{2} [Δ*ω*_{int}(*T*)], which are independent of the substrate. For the measured temperature-dependent Raman shifts in this work, the discrepancy in the frequency shifts between suspended and supported MoS_{2} originates only from the TEC mismatch-induced frequency shift between MoS_{2} and the substrate. Therefore, after subtracting Δ*ω*^{S}(*T*), the obtained values for suspended and supported MoS_{2} should be the same [Δ*ω*_{int}(*T*)]:

Using Equation (6), the value of can be deduced if we can obtain and However, the TEC mismatch-induced frequency shift for suspended MoS_{2} is challenging to experimentally determine. Because the MoS_{2} flake that surrounds the suspended MoS_{2} zone is still attached to the substrate, the TEC mismatch-induced strain can affect the Raman shift of suspended MoS_{2} to a certain extent.

Numerical simulations based on finite element theory (FET) provide a route to obtaining the thermal strain in suspended MoS_{2}. For the further study of the distribution of the thermal strain field, thermal strains at different temperatures were solved. In order to solve the FET simulation, the TECs for SiO_{2} and MoS_{2} should be provided as material parameters. The is adopted from the literature, whereas is identified in this work. In the first step, we can use the previously obtained using first-principles calculation in the simulations^{[36]}. The simulation results are presented in Supplementary Figure 1. It is assumed that the thermal strain is zero in the MoS_{2} samples at room temperature (*T*_{0} = 293 K). In fact, the strain distribution obtained using the FET simulations is composed of two components, namely, the strain due to the thermal expansion of the MoS_{2} layer and the strain induced by the TEC mismatch between MoS_{2} and the substrate. In order to obtain the strain induced by the TEC mismatch, FET simulations were also performed on a bare MoS_{2} flake (see Supplementary Figure 2), which is used to subtract the strain obtained based on the film-substrate model illustrated in Figure 1. The obtained TEC mismatch-induced strains *ε*(*T*) for the suspended and supported MoS_{2} are listed in Table 1. As demonstrated in the literature, the relationship between the TEC-induced strain and Raman shift can be expressed as^{[35]}:

Table 1

Simulated strain and the corresponding Raman shifts of the mode for suspended and supported MoS_{2} at selected temperatures

T (K) | 100 | 200 | 300 | 400 | 500 |
---|---|---|---|---|---|

ε_{sus} (%) | 0.005434 | 0.004523 | -0.0004271 | -0.007408 | -0.01319 |

ε_{sup} (%) | 0.006833 | 0.005673 | -0.0005339 | -0.009233 | -0.01640 |

(cm^{-1}) | -0.7227 | -0.6016 | 0.05680 | 0.9853 | 1.755 |

(cm^{-1}) | -0.9088 | -0.7545 | 0.07101 | 1.228 | 2.182 |

Therefore, the thermal strain-induced Raman shift can be obtained using Equation (7). The calculated TEC mismatch-induced strain and corresponding Raman shifts are listed in Supplementary Table 2. By bringing the and calculated by Equation (7) into Equation (6), it is found that the terms on the left- and right-hand sides cannot be consistent. This implies that the reported in previous work is inconsistent with the experimental results in our work. Therefore, in order to meet the requirements for Equation (6), a numerical inversion method was employed to select an optimum TEC of MoS_{2}. A flowchart for the numerical inversion procedure is plotted in Supplementary Figure 3.

With the help of the numerical inversion process, the proper TEC of monolayer MoS_{2} that satisfies Equation (6) was obtained. Employing the calculated , the simulation results for 100, 293 and 500 K are plotted in Figure 5 to illustrate the typical evolution of the strain distribution in the suspended and supported MoS_{2}. As shown in Figure 5A and B, the strain in both two MoS_{2} samples is zero at room temperature. Figure 5C and D show the strain of SUP-MoS_{2} and SUS-MoS_{2} at 100 K, respectively. It can be seen that the thermal strain in SUP-MoS_{2} caused by the thermal stress is uniform, while the deformation on the SUS-MoS_{2} mainly occurs on the central circular microhole and gradually decreases in the annular direction with a weak change. From the simulation results, it can be concluded that MoS_{2} sustains compressive strain. The deformation of SUS-MoS_{2} is larger because of the binding effect without the substrate. Because the TEC of MoS_{2} is larger than that of SiO_{2}, MoS_{2} shrinks faster with decreasing temperature and the deformation of MoS_{2} is inhibited by SiO_{2}. Therefore, the strain in SUS-MoS_{2} is larger than that of SUP-MoS_{2}. Figure 5E and F show the strain of SUP-MoS_{2} and SUS-MoS_{2} at 500 K. From the simulation results, it can be concluded that MoS_{2} experiences suppressed tensile strain. Similarly, the SUS-MoS_{2} deformation is greater due to the absence of the binding force of the substrate.

Figure 5. Numerical simulation results of supported and suspended MoS_{2}: (A), (C), (E) corresponding to the strain of SUP-MoS_{2} at 293, 100 and 500 K, respectively; (B), (D), (F) corresponding to the strain of SUS-MoS_{2} at 293, 100 and 500 K, respectively.

Using the same that was adopted in Figure 5, FET simulations were also performed on a bare MoS_{2} flake at different temperatures (see Supplementary Figure 4). By employing the simulated thermal strain in bare MoS_{2}, the TEC mismatch-induced strains for suspended and supported MoS_{2} were calculated. Then, by employing Equation (7), the frequency shifts of the mode for suspended and supported MoS_{2} are calculated and listed in Table 1.

The suitable obtained by the combination of the numerical simulation and Raman spectroscopy is plotted in Figure 6. One can see that the sign of is positive in the test temperature range. As shown in Table 2, the value of the obtained in this work is close to the values reported in the literature. Taking the TEC at room temperature for example, the obtained in this work is 7.13 (10^{-5} K^{-1}), while Ding *et al*.^{[12]} reported an of just 2.44 (10^{-5} K^{-1}) obtained by DFPT calculation. In contrast, the obtained in this work is in good agreement with previous results estimated experimentally. Late *et al*.^{[29]} reported a room-temperature of 8.2 (10^{-5} K^{-1}) obtained by combining temperature-dependent Raman spectroscopy and first-principles calculations. In addition, it is found that the TEC of MoS2 is much larger than that of SiO2. Therefore, MoS2 suppresses a tensile stress from the substrate, whether the sample was cooled or heated.

Figure 6. TEC obtained by combining temperature-dependent Raman spectroscopy and finite element simulations.

Table 2

Comparison of the TEC of MoS_{2} obtained from this work and those reported in the literature

Ref. | Method | TEC (10^{-5} K^{-1}) |
---|---|---|

Ding et al.^{[12]} (2015) | Density functional perturbation theory | 2.44 |

Late et al.^{[29]} (2014) | Raman + density functional theory | 8.20 |

Hu et al.^{[37]} (2018) | Electron energy-loss spectroscopy | 6.49 |

This work | Raman + finite element method | 7.13 |

In this work, we proposed a feasible method to assess the TEC of monolayer MoS_{2} by combining micro-Raman spectroscopy and numerical simulations. Suspended and supported MoS_{2} were systematically investigated using Raman spectroscopy in a temperature range from 77 to 557 K, which exhibited an obvious discrepancy in the evolution of Raman frequency shifts, demonstrating the critical effect due to the TEC mismatch between MoS_{2} and the substrate. Finite element simulations were used to calculate the TEC mismatch-induced thermal strain and Raman shift in the suspended and supported MoS_{2}. By matching the simulation results to the experimental results, the TEC of MoS_{2} was determined through a numerical inversion method. This method proposed in our work is a reasonable and adoptable route for determining the TEC of MoS_{2}, which can also be employed to obtain the TEC of 2D materials.

Design, writing review and editing: Yang Y, Long LC

Data analysis: Lin ZT, Li RF

Data acquisition: Liu WG, Li YT, Zhu K

Sample fabrication: Tian SB

Availability of data and materialsNot applicable.

Financial support and sponsorshipThis work was supported by the National Key Research and Development Program of China (No. 2018YFB0703500; No.2016YFA0200800), the National Natural Science Foundation of China (No. 11704401; No.12074420; No.11674387; No.61905274), the Key Deployment Project of Centre for Ocean Mega-Research of Science, Chinese academy of science (No. COMS2020J03).

Conflicts of interestAll authors declared that there are no conflicts of interest.

Ethical approval and consent to participateNot applicable.

Consent for publicationNot applicable

Copyright© The Author(s) 2021.

1. Chhowalla M, Liu Z, Zhang H. Two-dimensional transition metal dichalcogenide (TMD) nanosheets.

DOIPubMed*Chem Soc Rev*2015;44:2584-6.2. Lv R, Robinson JA, Schaak RE, et al. Transition metal dichalcogenides and beyond: synthesis, properties, and applications of single- and few-layer nanosheets.

DOIPubMed*Acc Chem Res*2015;3:897.3. Huang X, Zeng Z, Zhang H. Metal dichalcogenide nanosheets: preparation, properties and applications.

DOIPubMed*Chem Soc Rev*2013;42:1934-46.4. Chhowalla M, Shin HS, Eda G, Li LJ, Loh KP, Zhang H. The chemistry of two-dimensional layered transition metal dichalcogenide nanosheets.

DOIPubMed*Nat Chem*2013;5:263-75.5. Ding Y, Wang Y, Ni J, Shi L, Shi S, Tang W. First principles study of structural, vibrational and electronic properties of graphene-like MX2 (M=Mo, Nb, W, Ta; X=S, Se, Te) monolayers.

DOI*Physica B Condens Matter*2011;406:2254-60.6. Mak KF, Lee C, Hone J, Shan J, Heinz TF. Atomically thin MoS

DOI_{2}: a new direct-gap semiconductor.*Phys Rev Lett*2010;105:136805.7. Radisavljevic B, Radenovic A, Brivio J, Giacometti V, Kis A. Single-layer MoS

DOI_{2}transistors.*Nat Nanotechnol*2011;6:147-50.8. Yu Y, Yu Y, Xu C, et al. Engineering substrate interactions for high luminescence efficiency of transition-metal dichalcogenide monolayers.

DOI*Adv Funct Mater*2016;26:4733-9.9. Dai Z, Liu L, Zhang Z. Strain engineering of 2D materials: issues and opportunities at the interface.

DOI*Adv Mater*2019;31:e1805417.10. Yan Z, Liu G, Khan JM, Balandin AA. Graphene quilts for thermal management of high-power GaN transistors.

DOIPubMed*Nat Commun*2012;3:827.11. Sevik C. Assessment on lattice thermal properties of two-dimensional honeycomb structures: Graphene, h-BN, h-MoS

DOI_{2}, and h-MoSe_{2}.*Phys Rev B*2014;89.12. Ding Y, Xiao B. Thermal expansion tensors, Grüneisen parameters and phonon velocities of bulk MT

_{2}(M = W and Mo; T = S and Se) from first principles calculations.*RSC Adv*2015;5:18391-400.13. Huang LF, Gong PL, Zeng Z. Correlation between structure, phonon spectra, thermal expansion, and thermomechanics of single-layer MoS

DOI_{2}.*Phys Rev B*2014;90.14. Yuan J, Lv Z, Lu Q, Cheng Y, Chen X, Cai L. First-principles study of the phonon vibrational spectra and thermal properties of hexagonal MoS

DOI_{2}.*Solid State Sciences*2015;40:1-6.15. Liang L, Zhang J, Sumpter BG, Tan QH, Tan PH, Meunier V. Low-frequency shear and layer-breathing modes in Raman scattering of two-dimensional materials.

DOIPubMed*ACS Nano*2017;11:11777-802.16. Wang Y, Cong C, Qiu C, Yu T. Raman spectroscopy study of lattice vibration and crystallographic orientation of monolayer MoS

DOIPubMed_{2}under uniaxial strain.*Small*2013;9:2857-61.17. Saigal N, Wielert I, Čapeta D, et al. Effect of lithium doping on the optical properties of monolayer MoS

DOI_{2}.*Appl Phys Lett*2018;112:121902.18. Huang X, Zhang L, Liu L, et al. Raman spectra evidence for the covalent-like quasi-bonding between exfoliated MoS

DOI_{2}and Au films.*Sci China Inf Sci*2021;64.19. Mouri S, Matsuda K, Nanishi Y, Araki T. Thermal conductivity of van der Waals hetero-bilayer of MoS

DOI_{2}/MoSe_{2}.*Appl Phys Express*2020;13:075001.20. Zhang L, Lu Z, Song Y, et al. Thermal expansion coefficient of monolayer molybdenum disulfide using micro-raman spectroscopy.

DOIPubMed*Nano Lett*2019;19:4745-51.21. Lin Z, Liu W, Tian S, Zhu K, Huang Y, Yang Y. Thermal expansion coefficient of few-layer MoS

DOI_{2}studied by temperature-dependent Raman spectroscopy.*Sci Rep*2021;11:7037.22. Huang Y, Pan YH, Yang R, et al. Universal mechanical exfoliation of large-area 2D crystals.

DOI*Nat Commun*2020;11:2453.23. Baek SH, Choi Y, Choi W. Large-area growth of uniform single-layer MoS

DOIPubMedPMC_{2}thin films by chemical vapor deposition.*Nanoscale Res Lett*2015;10:388.24. Yang Y, Liu W, Lin Z, et al. Micro-defects in monolayer MoS

DOI_{2}studied by low-temperature magneto-Raman mapping.*J Phys Chem C*2020;124:17418-22.25. Chakraborty B, Matte HSSR, Sood AK, Rao CNR. Layer-dependent resonant Raman scattering of a few layer MoS

DOI_{2}: Raman scattering of a few layer MoS_{2}.*J Raman Spectrosc*2013;44:92-6.26. Tian S, Yang Y, Liu Z, et al. Temperature-dependent Raman investigation on suspended graphene: Contribution from thermal expansion coefficient mismatch between graphene and substrate.

DOI*Carbon*2016;104:27-32.27. Huang X, Gao Y, Yang T, Ren W, Cheng HM, Lai T. Quantitative analysis of temperature dependence of raman shift of monolayer WS2.

DOIPubMedPMC*Sci Rep*2016;6:32236.28. Chen Y, Wen W, Zhu Y, et al. Temperature-dependent photoluminescence emission and Raman scattering from Mo1-x W x S2 monolayers.

DOIPubMed*Nanotechnology*2016;27:445705.29. Late DJ, Shirodkar SN, Waghmare UV, Dravid VP, Rao CN. Thermal expansion, anharmonicity and temperature-dependent Raman spectra of single- and few-layer MoSe

DOI_{2}and WSe_{2}.*Chemphyschem*2014;15:1592-8.30. Zouboulis ES, Grimsditch M. Raman scattering in diamond up to 1900 K.

DOIPubMed*Phys Rev B Condens Matter*1991;43:12490-3.31. Su L, Yu Y, Cao L, Zhang Y.

DOIIn situ monitoring of the thermal-annealing effect in a monolayer of MoS_{2}.*Phys Rev Applied*2017;7.32. Chakraborty B, Bera A, Muthu DVS, Bhowmick S, Waghmare UV, Sood AK. Symmetry-dependent phonon renormalization in monolayer MoS

DOI_{2}transistor.*Phys Rev B*2012;85.33. Iqbal MW, Shahzad K, Akbar R, Hussain G. A review on Raman finger prints of doping and strain effect in TMDCs.

DOI*Microelectron Eng*2020;219:111152.34. Yoon D, Son YW, Cheong H. Negative thermal expansion coefficient of graphene measured by Raman spectroscopy.

DOIPubMed*Nano Lett*2011;11:3227-31.35. McCreary A, Ghosh R, Amani M, et al. Effects of uniaxial and biaxial strain on few-layered terrace structures of MoS

DOIPubMed_{2}grown by vapor transport.*ACS Nano*2016;10:3186-97.36. Zhang H, Wu Y. Electronic, thermal expanding, and optical absorption properties of transition metal dichalcogenides: a first-principles study.

DOI*J Wuhan Univ Technol-Mat Sci Edit*2018;33:1355-9.37. Hu X, Yasaei P, Jokisaari J, Öğüt S, Salehi-Khojin A, Klie RF. Mapping thermal expansion coefficients in freestanding 2D materials at the nanometer scale.

DOIPubMed*Phys Rev Lett*2018;120:055902.

Yang Y,
Lin Z,
Li R,
Li Y,
Liu W,
Tian S,
Zhu K,
Long L. Thermal expansion coefficient of monolayer MoS_{2} determined using temperature-dependent Raman spectroscopy combined with finite element simulations.
* Microstructures* 2021;1:2021002.
http://dx.doi.org/10.20517/microstructures.2021.02

387

72

0

0

0

Full-Text Views Each Month

PDF Downloads Each Month

© 2016-2021 OAE Publishing Inc., except certain content provided by third parties

## Comments

Comments must be written in English. Spam, offensive content, impersonation, and private information will not be permitted. If any comment is reported and identified as inappropriate content by OAE staff, the comment will be removed without notice. If you have any queries or need any help, please contact us at support@oaepublish.com.